3How much reinforcement? Weight fractionUsed in manufacture.May refer to fibre or resin - 'GRP' manufacturers will specify a glass content of (e.g.) 25 wt%; a prepreg supplier might give a resin content of 34 wt%.Volume fractionUsed in design to calculate composite properties. Almost always refers to fibre content.
4Weight fraction volume fraction conversion For the special case of a two-component composite (eg fibre and matrix):
6Maximum fibre volume fraction A composite cannot contain 100% fibre. Maximum volume fraction could be achieved only if unidirectional fibres are hexagonally ‘close packed’ - ie all fibres are touching.
7Maximum fibre volume fraction The triangular unit cell has area 3 R2.The unit cell contains an area of fibre (three 60o segments) equal to pR2 / 2
8Maximum fibre volume fraction In a unidirectional fibre composite, the fibre area fraction is the same as the fibre volume fraction, so:
9Maximum fibre volume fraction Theoretically, a unidirectional fibre composite could have Vf ≈ 90%. In practice, fibres cannot be perfectly aligned.Maximum volume fraction depends both on the fibre form and method of manufacture - for a unidirectional fibre composite: Vf ≈ 60-70%.
10Maximum fibre volume fraction For other forms of reinforcement, maximum volume fraction also depends on the detailed arrangement of the fibres.The following values are typical:stitched ‘non-crimp’ 0.6woven fabric random (chopped strand mat)
11How much fibre?Commercial reinforcements are characterised by their areal weight (Aw). This is simply the weight (usually given in g) of 1 m2 of the reinforcement. Aw depends on many factors - fibre density, tow or bundle size, weave style, etc.Aw may range from 50 g/m2 or less (for lightweight surfacing tissues), up to more than 2000 g/m2 for some heavyweight non-crimp fabrics.
12Laminate thicknessThe thickness of a composite laminate depends on the amount of reinforcement and the relative amount of resin which has been included.For a given quantity of reinforcement, a laminate with a high fibre volume fraction will be thinner than one with a lower fibre volume fraction, since it will contain less resin.
13Laminate thickness high matrix content low fibre content Two laminates, both containing 5 plies of reinforcement:fibrematrixhigh matrix contentlow fibre content= thick laminatelow matrix contenthigh fibre content= thin laminate
14Laminate thicknessFibre volume fraction is thus inversely proportional to laminate thickness.If the fibre content and laminate thickness are defined, we can calculate the fibre volume fraction:If the fibre content and volume fraction are defined, we can calculate the laminate thickness:
17Example calculations 1. What will be the thickness of a laminate consisting of 2 layers of 450 g/m2 chopped strand mat if a resin to glass ratio (by weight) of 2:1 is used? 2. What fibre volume fraction is achieved if 3 layers of 800 g/m2 glass woven roving are compression-moulded to a thickness of 2 mm?
19'Rules of Mixtures' are mathematical expressions which give some property of the composite in terms of the properties, quantity and arrangement of its constituents.They may be based on a number of simplifying assumptions, and their use in design should tempered with extreme caution!
20Density For the special case of a fibre-reinforced matrix: since Vf + Vm = 1
21Rule of mixtures density for glass/epoxy composites rfrm
23Unidirectional plyUnidirectional fibres are the simplest arrangement of fibres to analyse.They provide maximum properties in the fibre direction, but minimum properties in the transverse direction.fibre directiontransverse direction
24Unidirectional plyWe expect the unidirectional composite to have different tensile moduli in different directions.These properties may be labelled in several different ways:E1, E||E2, E
25Unidirectional plyBy convention, the principal axes of the ply are labelled ‘1, 2, 3’. This is used to denote the fact that ply may be aligned differently from the cartesian axes x, y, z.312
26Unidirectional ply - longitudinal tensile modulus We make the following assumptions in developing a rule of mixtures:Fibres are uniform, parallel and continuous.Perfect bonding between fibre and matrix.Longitudinal load produces equal strain in fibre and matrix.
27Unidirectional ply - longitudinal tensile modulus E1 = Ef Vf + Em ( 1-Vf )Note the similarity to the rules of mixture expression for density.In polymer composites, Ef >> Em, soE1 Ef Vf
28This rule of mixtures is a good fit to experimental data (source: Hull, Introduction to Composite Materials, CUP)
29Unidirectional ply - transverse tensile modulus LfLmThe simplified model ‘lumps’ fibre and matrix together, and assumes that both components experience the same stress:or
30Note that E2 is not particularly sensitive to Vf. If Ef >> Em,E2 Em / (1-Vf)Note that E2 is not particularly sensitive to Vf.If Ef >> Em, E2 is almost independent of fibre property:
31carbon/epoxyglass/epoxyThe transverse modulus is dominated by the matrix, and is virtually independent of the reinforcement.
32The transverse rule of mixtures is not particularly accurate, due to the simplifications made - Poisson effects are not negligible, and the strain distribution is not uniform:(source: Hull, Introduction to Composite Materials, CUP)
33Generalised rule of mixtures for tensile modulus E = hL ho Ef Vf + Em (1-Vf )hL is a length correction factor. Typically, hL 1 for fibres longer than about 10 mm.ho corrects for non-unidirectional reinforcement: